Weitere Artikel dieser Ausgabe durch Wischen aufrufen
Manuscript submitted September 16, 2014.
To produce high-quality ingot cast steel with a better surface quality, it would be beneficial for the uphill teeming process if a much more stable flow pattern could be achieved in the runners. Several techniques have been utilized in the industry to try to obtain a stable flow of liquid steel, such as a swirling flow. Some research has indicated that a swirl blade inserted in the horizontal and vertical runners, or some other additional devices and physics could generate a swirling flow in order to give a lower hump height, avoid mold flux entrapment, and improve the quality of the ingot products, and a new swirling flow generation component, TurboSwirl, was introduced to improve the flow pattern. It has recently been demonstrated that the TurboSwirl method can effectively reduce the risk of mold flux entrapment, lower the maximum wall shear stress, and decrease velocity fluctuations. The TurboSwirl is built at the elbow of the runners as a connection between the horizontal and vertical runners. It is located near the mold and it generates a tangential flow that can be used with a divergent nozzle in order to decrease the axial velocity of the vertical flow into the mold. This stabilizes flow before the fluid enters the mold. However, high wall shear stresses develop at the walls due to the fierce rotation in the TurboSwirl. In order to achieve a calmer flow and to protect the refractory wall, some structural improvements have been made. It was found that by changing the flaring angle of the divergent nozzle, it was possible to lower the axial velocity and wall shear stress. Moreover, when the vertical runner and the divergent nozzle were not placed at the center of the TurboSwirl, quite different flow patterns could be obtained to meet to different requirements. In addition, the swirl numbers of all the cases mentioned above were calculated to ensure that the swirling flow was strong enough to generate a swirling flow of the liquid steel in the TurboSwirl.
Bitte loggen Sie sich ein, um Zugang zu diesem Inhalt zu erhalten
Sie möchten Zugang zu diesem Inhalt erhalten? Dann informieren Sie sich jetzt über unsere Produkte:
D. J. Hurtuk: ASM Int., 2008, vol. 15, pp. 911-917.
R. Eriksson, L. Jonsson, and P.G. Jönsson (2004) ISIJ Int. 8(44):1358-1365. CrossRef
S. Yokoya, Y. Asako, S. Hara and J. Szekely: ISIJ Int., 1994, vol. 34, no. 11, pp. 883-888. CrossRef
S. Yokoya, S. Takagi, M. Iguchi, Y. Asako, R. Westof and S. Hara: ISIJ Int., 1998, vol. 38, no. 38, pp. 827-833. CrossRef
S. Yokoya, S. Takagi, K. Tada, M. Iguchi, K. Marukawa and S. Hara: ISIJ Int., 2001, vol. 41, no. 10, pp. 1201-1207. CrossRef
S. Yokoya, S. Takagi, M. Iguchi, K. Marukawa, W. Yasugaria and S. Hara: ISIJ Int., 2000, vol. 40, no. 6, pp. 584-588. CrossRef
L. Hallgren, S. Takagi, R. Eriksson, S. Yokoya and P.G. Jönsson: ISIJ Int., 2006, vol. 46, no. 11, pp. 1645-1651. CrossRef
L. Hallgren, S. Takagi, A. Tilliander, S. Yokoya and P.G. Jönsson: Steel Res. Int., 2007, vol. 78, no. 3, pp. 254-259.
Z. Zhang, S. Yokoya, A. Tilliander and P. G. Jönsson: ISIJ Int., 2010, vol. 50, no. 12, pp. 1756-1762. CrossRef
L. Hallgren, A. Tilliander, S. Yokoya, P.G. Jönsson and S. Hagman: ISIJ Int., 2010, vol. 50, no. 12, pp. 1763-1769. CrossRef
Z. Tan, M. Ersson and P.G. Jönsson: ISIJ Int., 2012, vol. 52, no. 6, pp. 1066-1071. CrossRef
Y. Yang, P.G. Jönsson, Z. Su, J. He and K. Nakajima: Steel Res. Int., 2015, vol. 86, no. 4, pp. 361-374. CrossRef
Y. Yang, P.G. Jönsson, M. Ersson and K. Nakajima: Steel Res. Int., 2015, vol. 86, no. 4, pp. 341-360. CrossRef
G. Solorio-Diaz, R. D. Morales, J. Palafax-Ramos, L. Garcia-Demedices and A. Ramos-Banderas: ISIJ Int., 2004, vol. 44, no. 6, pp. 1014-1032. CrossRef
G. Solorio-Diaz, R. D. Morales and A. Ramos-Banderas: Int. J. Heat Mass Tran., 2005, vol. 48, pp. 3574-3590. CrossRef
G. Solorio-Diaz, R. D. Morales, J. Palafax-Ramos and A. Ramos-Banderas: ISIJ Int., 2005, vol. 45, no. 8, pp. 1129-1137. CrossRef
G. Solorio-Diaz, R. Davlia-Morales, J. Barreto-Sandoval, H. J. Vergara-Hernandez, A. Ramos-Banderas and S. R. Galvan: Steel Res. Int., 2013, vol. 84, no. 9999, pp. 1-12.
Hsu FY, Jolly MR, Campbell J (2006) Int. J. Cast Metal Res. 19(1):38-44. CrossRef
Z. Tan, M. Ersson, P. Lidegran and P.G. Jönsson: Steel Res. Int., 2013, vol. 84, no. 9, pp. 837-844. CrossRef
Z. Tan, M. Ersson and P.G. Jönsson: ISIJ Int., 2011, vol. 51, no. 9, pp. 1461-1467. CrossRef
B. E. Launder and D. B. Spalding: Comput. Method Appl. M., 1974, vol. 3, pp. 269-289. CrossRef
Versteeg HK, Malalasekera W (2007) An Introduction to Computational Fluid Dynamics: The Finite Volume Method, 2nd edition. Pearson Education Limited, Essex
D. M. Driver and H. L. Seegmiller: AIAA J., 1985, vol. 23, no. 2, pp. 163-171. CrossRef
O. Kitoh: J. Fluid Mech., 1991, vol. 225, pp. 445-479. CrossRef
H. J. Sheen, W. J. Chen, S. Y. Jeng and T. L. Huang: Exp. Therm. Fluid Sci., 1996, vol. 12, pp. 444-451. CrossRef
I. Celik, U. Ghia, P. J. Roache, C. J. Freitas, H. Coleman and P. E. Raad (2008) J. Fluid Eng. T., vol. 130, no. 7, pp. 078001-078011.
- Effect of TurboSwirl Structure on an Uphill Teeming Ingot Casting Process
- Springer US
in-adhesives, MKVS, Hellmich GmbH/© Hellmich GmbH, Neuer Inhalt/© momius | stock.adobe.com